Comparison of resin composite restorations microleakage:
An in-vitro study
Horieh Moosavi1, Fatemeh Maleknejad Yazdi1, Fatemeh Velayati Moghadam1*, Saherh Soltani2
1Dental Material Research Center and Operative Dentistry Department, Dental School, Mashhad University of Medical Sciences, Mashhad, Iran
2Dentist, Mashhad, Iran Email: *Velayatimf@mums.ac.ir
Received 8 March 2013; revised 25 April 2013; accepted 8 May 2013
Copyright © 2013 Horieh Moosavi et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
The aim of this study was to compare the microleak- age of total-etch and self-etch adhesives by three me- thods including dye extraction, dye penetration and fluid filtration with determining the correlation value among these techniques. Seventy-two premolar teeth were selected for this in vitro study and Class 5 cavi- ties were prepared on the buccal surface of these at the cemento-enamel junction area. It was applied for half of these cavities, Optibond Solo Plus (OSP) (two- step etch & rinse) and another half, Optibond All-in- One (OA) (one-step self-etch) and then all of them were restored with a light cure resin composite; Her- culite XRV. Then samples were divided randomly into three subgroups based on the method of micro- leakage measurement (n = 12). In the first pair group, leakage was assessed by the dye extraction method. Dye penetration and fluid filtration methods were used in the second and third pair groups for the same purpose respectively. Data were analyzed by Paired t-test and Wilcoxon test and correlation coefficients (α = 0.05). There was no significant difference in the dye extraction (P = 0.657) and dye penetration (P = 0.732) methods between the microleakage of total- etch and self-etch adhesives. Microleakage of self-etch adhesive in fluid filtration technique was significantly more than total-etch adhesive (P = 0.012). No signifi- cant correlation was found among the results ob- tained with the three methods of microleakage eva- luation. Adhesive systems showed variously behave in different methods of microleakage assessment.
Keywords:Dye Extraction; Dye Penetration; Fluid
One of the esthetic materials which are used for restora- tion of Class V caries lesions is a resin composite with various dentine bonding systems which adhering the re- sin composite to tooth . An important factor in the success of the RC restorations is the properties of adhe- sive bonding agents. Resin-based adhesive systems can be classified in either the etch-and-rinse (ER) systems or the self-etch (SE) systems. The disadvantages of the ER systems are the technique sensitivity and the likely dis- crepancy between the extent of demineralization and monomer infiltration  and subsequent degradation of these adhesives when they are exposed to the mouth en- vironment during passing time [3,4]. The key advantages of SE adhesives are their easy and fast application pro- cedures . This approach significantly reduces techni- cal sensitivity. Infiltration of adhesive occurs simultane- ously with the etch process; therefore the discrepancy be- tween both processes is low and less time consuming [6, 7]. Knowing the success and longevity of various adhe- sives enables practitioners to choose the most appropriate material for the clinical use. The information on the bond- ing effectiveness of adhesives in laboratory conditions indicated that the bond strength of the all-in-one systems to enamel and dentin is not as high as other adhesive systems [8,9]. The cavity extends below the cemento- enamel junction (CEJ) with the margins in dentin; mi- croleakage, gap formation, and inappropriate adhesion to dentin remain considerable problems . The natural structure of dentin such as organic material content, the existence of liquid and odontiblastic branches in dentin, and the formation of the smear layer, are factors prevent- ing acquisition of a strong and durable bond [11,12]. An adhesive restoration may not attach properly to the etched dentineand forming marginal gap and microleakage . Marginal microleakage of restorations and the transmis-
sion of bacteria, liquids, and molecules between the cav- ity surface and the restorative material result in hyper- sensitivity, secondary caries, pulp stimulation, and mar- ginal discoloration [14-17]. There are a lot of studies were done on the microleakage of recent generation of adhesives which generally including Class V composite restorations. Different leakage tracers such as methylene blue, silver nitrate or basic fuchsin were used in these studies and profundity of dye was detected in each sam- ple for resin-dentin interface . In addition to the older methods like fluid filtration and dye penetration, it is ne- cessary to compare other microleakage test like dye ex- traction for composite resin restorations with them. In this method, methylene blue dilution in nitric acid was assessed by spectrophotometer with wavelength of 550 nm . Similarly to the previous studies on themicro- leakage evaluation of dentine adhesives [19-21], in this study, in addition to the common methods like fluid fil- tration and dye penetration, it was used dye extraction method and the correlations of these methods were deter- mined. Therefore, the purpose of this study was to com- pare the microleakage of a total-etchadhesive and a self- etchadhesive of one commercial brand by three methods including fluid filtration, dye penetration and dye extrac- tion, and determining the correlation among three meth- ods.
2. MATERIALS AND METHODS
Seventy-two freshly extracted human premolar teeth with no cares, filling, crack and abrasion was selected for
this in-vitro study. The teeth were extracted because of
periodontal or orthodontic problems and not extended than 3 months from the extraction. After debridement the crown and root of teeth by scaling and root planning in- struments, they were stored in 0.1% thymol solution at
4˚C. The thymol solution was changed to normal saline
one week before use. Class V cavities with 3 mm mesio- distal width, 1.5 mm axial depth and 2 mm occluso gin- givally length were prepared at the cement-enamel junc- tion on the buccal surface of teeth. The occlusal margin of the cavity was located on the enamel and the gingival
margin was located on the cementum. After cleaning the prepared cavities with flour of pumice and prophylactic rubber cup, half of the samples were treated randomly with Opti Bond Solo Plus (Kerr, Orange, USA) a total- etch adhesive and half of them were applied with Opti Bond All-in-One (Kerr, Orange, USA) a self-etch adhe- sive. Adhesives were used according to the manufac- turer’s instruction. After application of the adhesive sys- tems, prepared cavities were filled with a micro hybrid light cure resin composite Herculite XRV (Kerr, USA) incrementally in two 0.75 mm layers and each increment was cured for 20 seconds. The intensity of light curing
unit was 800 mW/cm2. Materials, chemical compositions
and clinical application were used in this study listed in
After 24 hours, the restorations were finished and pol- ished. The samples of each adhesive was randomly di- vided into three groups (each 24) based on the method used for measuring the microleakage. Another operator measered the samples microleakage with below proto- cols:
Dye extraction method: it was used to measure the mi- croleakage in restoration-dentin interface for total-etch and self-etch adhesive subgroups (n = 24). First the sam- ples were covered with 1 mm of restoration margins with two layers of nail varnish, the apices of roots were sealed with sticky wax and immersed in the 2% methylene blue solution for 24 hours. After 24 hours, the samples were rinsed under tap water for 30 minutes and nail varnish was removed by polishing disks. Then, for uses of spec- trophotometer, the samples were put in vials containing 65 wt% nitricacid for 3 days to let methylene blue within restorationdentin interface diluted in nitric acid. It is nec-
essary to mention that there was 1000 μl acid volume in
each vial. The vials were centrifuged 14,000 rpm for 5
minutes and after that, 100 μl of the supernatant from
each was transferred to a plate. The dye absorption was measured by an automatic spectrophotometer at 550 nm using concentrated nitric acid as the blank. The results of the spectrophotometer indicate the light absorption of the methylene blue in the resin-dentin interface which is ac-
Table 1. Materials, manufacturers, chemical compositions and clinical applications used in this study.
Material name Manufacturer Chemical composition Clinical application
Optibond Solo Plus adhesive (OSP); Two-step total-etch adhesive
Kerr Corporation, Orange,
CA, USA HEMA, Bis GMA, Camphorquinone, Barium borosilicate, Sodium hexaflurosilicate, Ethanol
35% phosphoric acid for 15 s, rinse, removes excess water. Apply bonding for 20 s, briefly air-dry, light-activate for 20 s.
Optibond All-in-One adhesive (OA); One-step self-etch adhesive
Kerr Corporation, Orange, CA, USA
HEMA, GPDM, Camphorquinone,
Co-monomers, Three nanosized fillers, Sodium hexaflurosilicate, Yttereium fluoride, Solvent-water, acetone, ethanol
Apply bonding for 20 s in two layers, gently air-dry, light-activate for 20 s.
Herculite XRV composite; (Micro-hybrid composite)
Kerr Corporation, Orange, CA, USA
Bis-GMA resin matrix, 79 wt% filler, Camphorquinone, etc.
tually showing the microleakage of the restoration. Dye penetration method: it is used to measure the mi- croleakage as the following way for two used adhesives (n = 24). First the samples were sealed like the first group and immersed in 2% methylene blue solution for 24 hours. After that, the samples were rinsed under tap water for 30 minutes. Then the samples were embedded in Epoxy Resin and restorations sectioned buccolingually through its mesiodistal center by a water-cooled diamond saw. Each section was assessed by a stereomicroscopeat 60× magnification to measure the microleakage. To mea- sure the microleakage in this study, a scale from 0 to 3 was used. Score 0 = no marginal leakage, Score 1 = dye penetration up to 1/2 depth of the cavity, Score 2 = dye penetration more than 1/2 depth of the cavity and Score 3 = dye penetration extending to the axial wall of the ca- vity.
Fluid filtration method: it is based on the evaluation of liquid transportation in the specimen, which was calcu- lated from the movement of bubbles. Fluid leaking through the restoration interface of the specimens was measured by displacement of an air bubble in an attached glass capillary. An oxygen tank with a manometer (for precise adjustment of pressure) was attached to set-up. A plastic tube must be connected to the oxygen source, and the end part should be connected to an erlen. A plastic tube was connected to a three-valve tube by a 0.5 cm × 2 cm long latex pipe. A syringe was connected to the lower side of the three-valve tube to make an air bubble th- rough the micro pipette. The upper side was connected to the specimens. The cyanoacrylate glue was smeared on all of the system connections (Inter Lock, Japan) and multiple layers of Para film strips were covered all of them (Parafilm “M”; Laboratory film, Chicago, IL). These strips seal the connections in tubes and ensure a strong connection. A diamond disk which was mounted on a low speed hand pice used to sectioning the roots from the crowns to 2 mm below the cemento-enamel junction (C.E.J). The pulpal soft tissue was removed and the area washed with a saline solution. A plexiglass sur- face was used as the base of the final crown segments. The camera was zoomed and focused on the macrograph to produce a sharp image. By opening the faucet and re- moving the syringe, the pass in there was a straight con- nection between the tooth and the fluid filtration system. The main oxygen tank faucet was opened and remained in a constant, exact pressure ratio during the experiment. Then the digital camera started capturing the steps in every 2 minutes (2, 4, 6, 8 min). All the process was re- peated for the system and all the data were saved to the P.C Hard Disc and the bubble movement was evaluated by the Photoshop software.
Data were analyzed by Paired t-test, Mann-Whitney, Pearson and Spearman tests. All statistical tests were run
at 5% significance level (P ≤ 0.05).
For comparing the microleakage of total-etch and self-
etch adhesives, Figure 1 was indicated that there was
more leakage in self-etch adhesive than total-etch adhe- sive for dye extraction method but using Paired t-test, there was no significant difference in microleakage be- tween the adhesives (P = 0.728).
According to the results illustrating in Figure 2, for
dye penetration method the microleakage of total-etch adhesive was more than self-etch adhesive while using- Mann-Whitney showed there was no significant differ- ence in the microleakages of the adhesives (P = 0.755).
Figure 3 was illustrated that in fluid filtration method,
the microleakage of self-etch adhesive was more than total-etch adhesive and by using Paired t-test, the micro- leakage of the two adhesives indicated a significant dif- ference (P = 0.002). Therefore, using fluid filtration me- thod to assess the microleakage, Optibond All-in-One (self-etch adhesive) had more leakage than Optibond Solo Plus (total-etch adhesive).
Figure 1. The comparisons of average microleakage in
total-etch and self-etch adhesives in dye extraction me- thod.
Figure 2. The comparison of average microleakage in
Figure 3. The comparison of average microleakage in
to-tal-etchand self-etchadhesives by fluid filtration method.
According to the Table 2 there were no significant
correlation between different methods of microleakage measurement, but there was a positive correlation be- tween them.
The main gold of this study was to compare the three methods for microleakage assessment including dye ex- traction (quantitative method), dye penetration (qualita- tive method) and fluid filtration (quantitative method), in Class V composite resin restorations with a total-etch and a self-etch adhesive from one manufacturer. The evalua- tion of microleakage is performed by different methods, such as air pressure, bacterial assessment, radioisotope studies, scanning electron microscopy, chemical identifi- ers, electrochemical studies, and measurement of dye penetration [11,22,23]. Some studies have reported that different methods of microleakage evaluation do not dif- fer in the final results [19,24]. To compare the average microleakage in Class V composite restorations, total- etch and self-etch adhesives were used such as previous studies [14-18]. Regarding the trend toward simplifica- tion, self-etch adhesives that combine the steps of etch- ing, priming and bonding into one solution have become common. These self-etch, seventh-generation adhesives also called all-in-one adhesives. All-in-one adhesives act as semi permeable membranes, consequential a hydro- lytic degradation of the resin-dentin interface . Com- parison of average microleakage in total-etch adhesive (Opti Bond Solo Plus) and self-etch adhesive (Optibond All-in-One) based on dye extraction and dye penetration methods indicated that the microleakage of both adhe- sives was not significantly different. Similarly to our
result, Brackett et al. also used dye penetration for the
microleakage in dentin margins and the results were in- dicated that there were no significant difference between self-etch adhesives and total-etch adhesive [15,17]. The adhesives in the current study included an etch-and-rinse
Table 2. Spearman’s rho and Pearson results for the correlation
between three methods of microleakage tests in experimental groups.
Method of microleakage assessment
coefficient P-value Dye extraction with Dye
penetration **SR = 0.048 P = 0.824
Dye extraction with
Fluid-Filtration *SR = 0.102 P = 0.637 Dye penetration with
Fluid-Filtration *PR = 0.165 P = 0.442
*Pearson correlation = PR; **Spearman correlation = SR.
one-bottle system and a mild self-etch adhesive system; both are different in the hybrid layer formation and bond- ing mechanism. The demineralization of dentin and ena- mel in mild self-etch adhesives occur using acidic prim- ers, so that some hydroxyapatite crystals exposed to aci- dic monomers remain around collagen fibrils in dentin. It is suggested that these remaining crystals have a chemi- cal reaction with functional monomers and can prevent marginal microleakage [6,25]. Some researchers have shown differences in the sealing ability of restoration margins between these adhesives [26,27]. The results of the current study are consistent with studies carried out by Mitsui and others  and Pradelle and others ; both researchers stated that etch-and-rinse and self-etch systems do not differ in dentin margin microleakage. In fluid filtration method of this study, the microleakage of self-etch adhesive was more significantly than total-etch adhesive. In contrast of our finding, it was indicated that Xeno III self-etch adhesive had less leakage than Prime & Bond NT total-etch adhesive using fluid filtration . This difference may be referred to the different self-etch and total-etch adhesives used in these studies and the la- boratory assembly. Incomplete bonded restorations may produce changes in fluid flow and microleakage . In the present study, more microleakage was observed in the self-etch adhesive than in the total-etch adhesive that is in agreement with those of Loguercio et al. study .
experimental self-etch adhesive containing GDM mono- mer and filler showed higher property in comparison of total-etch adhesive, indicating higher crosslink density accompanied by a probably in- crease the degree of con- version in the polymer network structure. For some pre- vious studies [14,15,17,35,36] only dye penetration me- thod was used to assess the microleakage of composite restorations. In the present study, like one previous study to evaluate the correlations among the three methods of microleakage assessment, fluid filtration method was defined as the control group and the correlations of the two other methods were assessed by it . Therefore, the study was not indicated any significant correlations between the qualitative method (dye penetration) and quantitative methods (fluid filtration and dye extraction) like the past paper  but there was a positive correla- tion between them. This finding may be due the different test set-up and separate samples prepared for each mi- croleakage assessment method. Additionally it is advis- able to use dye extraction methods instead of fluid filtra- tion since dye extraction gave the same results as fluid filtration but saved much laboratory time. In the future, it would be advisable to assess the sealing ability different adhesives with various methods and handling techniques for a long time and even in a situ study.
With the limitations of this study, it can be concluded that: Self-etch adhesive showed variously behave in dif- ferent methods of microleakage assessment and proved more microleakage than total-etch adhesive in this short time evaluation. There were no significant correlations between different methods of microleakage evaluation.
The authors would like to thank the research council of the Mashhad University of Medical Sciences which financially supported this study (protocol code 88455, Dental student thesis 2448).
 Hegde, M.N., Vyapaka, P. and Shetty, S. (2009) A com- parative evaluation of microleakage of three different newer direct composite resins using a self etching primer in class V cavities: An in vitro study. Journal of Conser- vative Dentistry, 12, 160-163.
 Moosavi, H., Moazzami, S.M., Loh, S. and Salari, S. (2010) Microleakage evaluation of core buildup compos- ite resins with total-etch and self-etch adhesive systems. Journal of Contemporary Dental Practice, 11, e009-e016.
 Hashimoto, M., Ohno, H., Kaga, M., Endo, K., Sano, H. and Oguchi, H. (2000) In vivo degradation of resin-dentin bonds in humans over 1 to 3 years. Journal of Dental Re- search, 79, 1385-1391.
 De Munck, J., Van Meerbeek, B., Yoshida, Y., Inoue, S., Vargas, M., Suzuki, K., Lambrechts, P. and Vanherle, G. (2003) Four-year water degradation of total-etch adhe- sives bonded to dentin. Journal of Dental Research, 82, 136-140. doi:10.1177/154405910308200212
 Ermis, R.B., Van Landuyt, K.L., Cardoso, M.V., De Munck, J., Van Meerbeek, B. and Peumans, M. (2012) Clinical effectiveness of a one-step self-etch adhesive in non-carious cervical lesions at 2 years. Clinical Oral In- vestigations, 16, 889-897.
 Van Meerbeek, B., De Munck, J., Yoshida, Y., Inoue, S., Vargas, M., Vijay, P., Van Landuyt, K., Lambrechts, P. and Vanherle, G. (2003) Buonocore memorial lecture. Adhesion to enamel and dentin: Current status and future challenges. Operative Dentistry, 28, 215-235.
 Wang, Y. and Spencer, P. (2005) Continuing etching of an all-in-one adhesive in wet dentin tubules. Journal of Dental Research, 84, 350-354.
 Van Landuyt, K.L., Mine, A., De Munck, J., Jaecques, S., Peumans, M., Lambrechts, P. and Van Meerbeek, B. (2009) Are one-step adhesives easier to use and better performing? Multifactorial assessment of contemporary one-step self-etching adhesives. Journal of Adhesive Den- tistry, 11, 175-190.
 Bradna, P., Vrbova, R., Dudek, M., Roubickova, A. and Housova, D. (2008) Comparison of bonding performance of self-etching and etch-and-rinse adhesives on human dentin using reliability analysis. Journal of Adhesive Den- tistry, 10, 423-429.
 Sadeghi, M. (2009) Influence of flowable materials on microleakage of nanofilled and hybrid class II composite restorations with LED and QTH LCUs. Indian Journal of Dental Research, 20, 159-163.
 Swift Jr., E.J., Triolo Jr., P.T., Barkmeier, W.W., Bird, J.L. and Bounds, S.J. (1996) Effect of low-viscosity res- ins on the performance of dental adhesives. American Journal of Dentistry, 9, 100-104.
 Unlu, N., Krakaya, S., Ozer, F. and Say, E. (2003) Re- ducing microleakage in composite resin restorations: An in vitro study. European Journal of Prosthodontic Re- storative Dentistry, 11, 171-175.
 Manuja, N. and Nagpal, R. (2012) Resin-tooth interfacial morphology and sealing ability of one-step self-etch ad- hesives: Microleakage and SEM study. Microscopy Re- search and Technique, 75, 903-909.
 Koliniotou-Koumpia, E., Dionysopoulos, P. and Koum- pia, E. (2004) In vitro evaluation of microleakage from composites with new dentin adhesives. Journal of Oral Rehabilitation, 31, 1014-1022.
 Bracket, W.W., Haisch, L.D., Pearce, M.G. and Brackett, M.G. (2004) Microleakage of Class V resin composite restorations placed with self-etching adhesives. Journal of Prosthetic Dentistry, 91, 42-45.
 Gregoire, G., Guignes, P.H. and Millas, A. (2005) Effect of self-etching adhesives and dentin permeability in a fluid flow model. Journal of Prosthetic Dentistry, 93, 56-
 Brackett, M.G., Brackett, W.W. and Haisch, L.D. (2006) Microleakage of Class V resin composites placed using self-etching resins: Effect of prior enamel etching. Quin- tessence International, 37, 109-113.
 Deliperi, S., Bardwell, D.N. and Wegley, C. (2007) Res- toration interface microleakage using one total-etch and three self-etch adhesives. Operative Dentistry, 32, 179-
 Camps, J. and Pashley, D. (2003) Reliability of the dye penetration studies. Journal of Endodontic, 29, 595-599. doi:10.1097/00004770-200309000-00012
 De Gee, A.J., WU, M.K. and Wesselink, P.R. (1994) Sealing properties of Ketac-Endo glass ionomer cement and AH26 root canal sealers. International Endodontic Journal, 27, 239-244.
 Pommel, L., Jacquot, B. and Camps, J. (2001) Lack of correlation among three methods for evaluation of apical leakage. Journal of Endodontics, 27, 347-350.
 Leevailoj, C., Cochran, A., Matis, B.A., Moore, B.K. and Platt, J.A. (2001) Microleakage of posterior packable resin compositeswith and without flowable liners. Opera- tive Dentistry, 26, 302-307.
 Jain, P. and Belcher, M. (2000) Microleakage of Class II resin based composite restorations with flowable compo- site in the proximal box. American Journal of Dentistry,
 Moosavi, H., Moghaddas, M.J., Ghoddusi, J. and Rajabi, O. (2010) Effects of two antioxidants on the microleak- age of resin-based composite restorations after nonvital bleaching. The Journal of Contemporary Dental Practice,
 Breschi, L., Mazzoni, A., Ruggeri, A., Cadenaro, M., Di- Lenarda, R. and De Stefano Dorigo, E. (2008) Dental ad- hesion review: Aging and stability of the bonded inter- face. Dental Materials, 24, 90-101.
 Mitsui, F.H., Bedran-de-Castro, A.K., Ritter, A.V., Car- doso, P.E. and Pimenta, L.A. (2003) Influence of load cycling onmarginal microleakage with two self-etching and two one-bottle dentin adhesive systems in dentin. Journal of Adhesive Dentistry, 5, 209-216.
 Pradelle-Plasse, N., Wenger, F., Picard, B. and Colon, P. (2004) Evaluation of microleakage of composite resin re- storationsby an electrochemical technique: The imped- ance methodology. Dental Materials, 20, 425-434.
 Vaidyanathan, T.K. and Vaidyanathan, J. (2009) Recent advances in the theory and mechanism of adhesive resin bonding to dentin: A critical review. Journal of Biomedi- cal Materials Research Part B: Applied Biomaterials, 88, 558-578. doi:10.1002/jbm.b.31253
 Loguercio, A.D., Bittencourt, D.D., Baratieri, L.N. and Reis, A. (2007) A 36-month evaluation of self-etch and etch-and-rinse adhesives in non-carious cervical lesions. The Journal of the American Dental Association, 138, 507-514.
 Khoroushi, M. and Aghelinejad, S. (2011) Effect of post- bleaching application of an antioxidant on enamel bond strength of three different adhesives. Medicina Oral, Pa- tología Oral y Cirugía Bucal, 16, e990-e996.
 Kubo, S., Kawasaki, K., Yokota, H. and Hayashi, Y. (2006) Five-year clinical evaluation of two adhesive sys- tems in non-carious cervical lesions. Journal of Dentistry,
 Peumans, M., De Munck, J., Van Landuyt, K., Lam- brechts, P. and Van Meerbeek, B. (2007) Five-year clini- cal effectiveness of a two-step self-etching adhesive. Jour- nal of Adhesive Dentistry, 9, 7-10.
 Park, J., Eslick, J., Ye, Q., Misra, A. and Spencer, P. (2011) The influence of chemical structure on the proper- ties in methacrylate-based dentin adhesives. Dental Ma- terials, 27,1086-1093. doi:10.1016/j.dental.2011.07.011
 Itoh, S., Nakajima, M., Hosaka, K., Okuma, M., Takaha- shi, M., Shinoda, Y., Seki, N., Ikeda, M., Kishikawa, R., Foxton, R.M. and Tagami, J. (2010) Dentin bond durabil- ity and water sorption/solubility of one-step self-etch ad- hesives. Dental Materials Journal, 29,623-630.
 Manhart, J., Yan Chen, H., Mehl, A., Weber, K. and Hichel, R. (2001) Marginal quality and microleakage of adhesive Class V restorations. Journal of Dentistry, 29,